4. Magnesium sulfate - ULB Halle: Online-Publikationen · PDF fileMagnesium sulfate 36 4....
Embed Size (px)
Transcript of 4. Magnesium sulfate - ULB Halle: Online-Publikationen · PDF fileMagnesium sulfate 36 4....
4. Magnesium sulfate Magnesium sulfate forms various hydrates in aqueous solution. Experiments have been conducted with two phases, the heptahydrate, MgSO4 • 7H2O, also referred to as epsomite, and the hexahydrate, MgSO4 • 6H2O, known as hexahydrite. A comprehensive study of the influence of additives on thermodynamics and kinetics of crystallization of magnesium sulfate hydrates is presented. Furthermore, phase transformations in pure and impure solutions have been studied, particularly with regard to induction times in dependence on the purity of the system or temperature, respectively. 4.1 Influence of additives on thermodynamics and kinetics of crystallization The effect of several additives on the solubility, metastable zone width, growth rate and on the crystal habit has been determined experimentally. For a better basis for discussion, certain additives have been chosen of which the influence on some features of the crystallization process had already been published (see e.g. /KARP84, NYV95/). Furthermore, all additives chosen may occur as solution by-products in actual industrial crystallization processes.
4.1.1 Solubility Due to the addition of an impurity, the solubility of a given substance my increase, decrease or not change at all within detectable limits. With magnesium sulfate, all three effects mentioned can be observed. The influence of twelve different additives on the solubility is qualitatively illustrated in Figure 4.1-1. Fig. 4.1-1. Influence of additives on the solubility of epsomite
CaSO4 • 2H2O
Na2B4O7 • 10H2O
NiSO4 • 6H2O Na2SO4
Ti = const.
FeSO4 • H2O
As can be taken from Figure 4.1-1, KCl is the only impurity that does not noticeably influence the solubility of epsomite. Some additives increase the solubility: KH2PO4, K2SO4, Na2B4O7 • 10H2O, NaOH However, most additives lead to a decrease in solubility: CaSO4 • 2H2O, FeSO4 • H2O, H2SO4, MgCl2, NaCl, Na2SO4, NiSO4 • 6H2O Quantitative solubility data can be found in the appendix / section 14.4 and 14.5.
4.1.2 Metastable zone width Additives might also exert an influence on the width of the metastable zone. Many cases of additives widening the metastable zone can be found in literature and only few examples are known in which an impurity decreases the metastable zone width. In Figure 4.1-2, the influence of twelve additives on the metastable zone width of magnesium sulfate solutions is illustrated. Since different amounts of additives are used, the respective amount is indicated in each column. The additives are listed in alphabetical order. Fig. 4.1-2. Influence of additives on the metastable zone width The metastable zone width, or in other words the maximum possible supercooling, can be distinctly influenced by additives (see Figure 4.1-2). In Figure 4.1-2 mean values of five measurements are shown, all of which have been carried out with the ultrasonic measuring technique. Most additives exert only little influence on the metastable zone
.7 2 w
0H 2O Na
. s up
width. However, two additives have a pronounced effect: borax (Na2B4O7 • 10H2O) and sodium hydroxide. The addition of borax causes a significant widening of the metastable region, whereas the addition of sodium hydroxide, i.e. the shift of pH into the alkaline region, reduces the maximum possible supercooling. Comprehensive data on the influence of these additives on the metastable zone width of magnesium sulfate solutions is shown in the appendix, section 14.6. In this section, solely further information about the effect of potassium chloride (KCl) and di-sodium tetraborate decahydrate (borax) will be given. Fig. 4.1-3. Influence of KCl on the maximum supercooling The influence of different amounts of KCl on the maximum supercooling is shown in Figure 4.1-3. In this diagram the cooling rate – which has been kept constant in all experiments – is depicted above the maximum possible supercooling. Although for all experiments thermostatic baths have been programmed with a cooling rate of 10 K / h, the actual cooling rate ranged from approximately 8 to 9 K / h. Nevertheless, the influence of variations in the cooling rate have been neglected. For pure magnesium sulfate solutions the maximum possible supercooling varies between 3.3 and 4.0 K. By the addition of KCl no distinct changes in the supercooling-behavior can be observed. Even amounts as high as 2 wt% KCl only have a negligible effect on the temperature at which nucleation takes place. Since the addition of KCl does not change the solubility of epsomite in aqueous solution within detectable limits, no significant effect of this additive on the metastable zone width is detected (see Figure 4.1-3). As already shown in Figure 4.1-2, borax distinctly influences the metastable zone width. In the following diagram, Figure 4.1-4, the maximum supercooling of aqueous magnesium
3 3,3 3,6 3,9 4,2 4,5 supercooling [K]
pure solution 0.5 wt% KCl 1 wt% KCl 2 wt% KCl
sulfate solutions in dependence of the impurity concentration is illustrated. Experiments have been carried out in the same manner as described for KCl and, again, an almost constant cooling rate is employed. The maximum supercooling increases significantly even with additive amounts as low as 0.1 wt%. Experiments have been conducted with additive- concentrations ranging from 0.1 to 5 wt% borax. Up to 5 wt% borax a continuous increase in the width of the metastable zone with increasing additive concentration can be observed. Fig. 4.1-4. Influence of borax on the maximum supercooling The influence of borax on the metastable zone width is also illustrated in Figure 4.1-5. Fig. 4.1-5. Influence of borax on the metastable zone width
2,5 3,5 4,5 5,5 6,5 7,5 8,5 supercooling [K]
pure solution 0.1 wt% borax 0.5 wt% borax 1 wt% borax 2 wt% borax 5 wt% borax
19 21 23 25 27 29 31 33 35 37 temperature [°C]
pure solution 2 wt% borax 5 wt% borax
The black line is the result obtained with the ultrasonic measuring technique for a pure magnesium sulfate solution. The medium gray and light gray lines represent results for solutions with 2 and 5 wt% borax, respectively. In each case, the ultrasonic velocity increases almost linearly with temperature. Only when nucleation starts, a sudden decrease of the ultrasonic velocity can be observed. Saturation and nucleation temperatures for each condition are marked with a black dot. The saturation temperature for pure solutions is 30.5°C. With increasing amount of borax, saturation as well nucleation temperatures are shifted towards lower temperatures. However, the influence of borax on the nucleation temperature is stronger than on the saturation temperature and therefore the metastable zone width broadens. The metastable zone width in dependence on the amount of borax is also emphasized by the striped field (see Figure 4.1-5). In addition, also experiments with varying cooling rates have been carried out with the same additives, KCl and borax. All solutions are saturated at approximately 30.5°C. A comparison between the maximum supercooling in pure and impure solutions in dependence on the cooling rate is presented in Figure 4.1-6. Fig. 4.1-6. Metastable zone width of pure and impure solutions for different cooling rates Both additives have been used in quantities of 0.5 wt% and mean values of five measurements are taken as basis for the diagram / Figure 4.1-6. On an average, solutions with KCl exhibit a slightly smaller metastable zone than pure solutions. In contrast to it, solutions with borax can be supercooled to a larger extent than pure solutions, independent of the cooling rate employed. It is also apparent from Figure 4.1-6, that the metastable zone is a function of the cooling rate. The metastable zone broadens with increasing cooling rate, for pure solutions as well as for solutions containing